IS 456 : 2000
PLAIN AND REINFORCED CONCRETE -
CODE OF PRACTICE
(Fourth Revision )
0 BIS 2000
BUREAU OF INDIAN STANDARDS
MANAK BHAVAN, 9 BAHADUR SHAH ZAFAR MARG
NEW DELHI 110002
July 2000 Price Rs 260.00
( Reaffirmed 2005 )
( Fourth Revision )
This Indian Standard (Fourth Revision) was adopted by the Bureau of Indian Standards, after the draft finalixed
by the Cement and Concrete Sectional Committee had been approved by the Civil Engineering Division Council.
This standard was first published in 1953 under the title ‘Code of practice for plain and reinforced concrete for
general building construction’ and subsequently revised in 1957. The code was further revised in 1964 and
published under modified title ‘Code of practice for plain and reinforced concrete’, thus enlarging the scope of
use of this code to structures other than general building construction also. The third revision was published in
1978, and it included limit state approach to design. This is the fourth revision of the standard. This revision
was taken up with a view to keeping abreast with the rapid development in the field of concrete technology and
to bring in further modifications/improvements in the light of experience gained while using the earlier version
of the standard.
This revision incorporates a number of important changes. The major thrust in the revision is on the following
a) In recent years, durability of concrete structures have become the cause of concern to all concrete
technologists. This has led to the need to codify the durability requirements world over. In this revision
of the code, in order to introduce in-built protection from factors affecting a structure, earlier clause on
durability has been elaborated and a detailed clause covering different aspects of design of durable
structure has been incorporated.
b) Sampling and acceptance criteria for concrete have been revised. With tbis revision acceptance criteria
has been simplified in line with the provisions given in BS 5328 (Part 4):1990 ‘Concrete: Part 4
Specification for the procedures to be used in sampling, testing and assessing compliance of concrete’.
Some of the significant changes incorporated in Section 2 are as follows:
All the three grades of ordinary Portland cement, namely 33 grade, 43 grade and 53 grade and sulphate
resisting Portland cement have been included in the list of types of cement used (in addition to other
types of cement).
The permissible limits for solids in water have been modified keeping in view the durability requirements.
The clause on admixtures has been modified in view of the availability of new types of admixtures
In Table 2 ‘Grades of Concrete’, grades higher than M 40 have been included.
It has been recommended that minimum grade of concrete shall be not less than M 20 in reinforced
concrete work (see also 6.1.3).
The formula for estimation of modulus of elasticity of concrete has been revised.
In the absenceof proper correlation between compacting factor, vee-bee time and slump, workability
has now been specified only in terms of slump in line with the provisions in BS 5328 (Parts 1 to 4).
Durability clause has been enlarged to include detailed guidanceconcerning the factors affecting durability.
The table on ‘Environmental Exposure Conditions’ has been modified to include ‘very severe’ and
‘extreme’ exposure conditions. This clause also covers requirements for shape and size of member,
depth of concrete cover, concrete quality,requirement againstexposure to aggressive chemical and sulphate
attack, minimum cement requirement and maximum water cement ratio, limits of chloride content, alkali
silica reaction, and importance of compaction, finishing and curing.
A clause on ‘Quality Assurance Measures’ has been incorporated to give due emphasis to good practices
Proper limits have been introduced on the accuracy of measuring equipments to ensure accurate batching
IS 456 : 2000
m) The clause on ‘Construction Joints’ has been modified.
n) The clause on ‘Inspection’ has been modified to give more emphasis on quality assurance.
The significant changes incorporated in Section 3 are as follows:
Requirements for ‘Fire Resistance’ have been further detailed.
The figure for estimation of modification factor for tension reinforcement used in calculation of basic
values of span to effective depth to control the deflection of flexural member has been modified.
Recommendations regarding effective length of cantilever have been added.
Recommendations regarding deflection due to lateral loads have been added.
Recommendations for adjustments of support moments in restrained slabs have been included.
In the detemination of effective length of compression members, stability index has been introduced to
determine sway or no sway conditions.
Recommendations have been made for lap length of hooks for bars in direct tension and flexural tension.
Recommendations regarding strength of welds have been modified.
Recommendations regarding cover to reinforcement have been modified. Cover has been specified
based~ondurability requirements for different exposure conditions. The term ‘nominal cover’ has been
introduced. The cover has now been specified based on durability requirement as well as for fite
The significant change incorporated in Section 4 is the modification-of the clause on Walls.The modified clause
includes design of walls against horizontal shear.
In Section 5 on limit state method a new clause has been added for calculation of enhanced shear strength of
sections close to supports. Some modifications have also been made in the clause on Torsion. Formula for
calculation of crack width has been-added (separately given in Annex P).
Working stress method has now been given in Annex B so as to give greater emphasis to limit state design. In
this Annex, modifications regarding torsion and enhanced shear strength on the same lines as in Section 5 have
Whilst the common methods of design and construction have been covered in this code, special systems of
design and construction of any plain or reinforced concrete structure not covered by this code may be permitted
on production of satisfactory evidence regarding their adequacy and safety by analysis or test or both
In this code it has been assumed that the design of plain and reinforced cement concrete work is entrusted to a
qualified engineer and that the execution of cement concrete work is carried out under the direction of a qualified
and experienced supervisor.
In the formulation of this standard, assistance has been derived from the following publications:
BS 5328-zPart 1 : 1991 Concrete : Part 1 Guide to specifying concrete, British Standards Institution
BS 5328 : Part 2 : 1991 Concrete : Part 2 Methods for specifying concrete mixes, British Standards
BS 5328 : Part 3 : 1990 Concrete : Part 3 Specification for the procedures to be used in producing and
transporting concrete, British Standards Institution
BS 5328 : Part 4 : 1990 Concrete : Part 4 Specification for the procedures to be used in sampling, testing
and assessing compliance of concrete, British Standards Institution
BS 8110 : Part 1 : 1985 Structural use of concrete : Part 1Code of practice for design and construction,
British Standards Institution
BS 8110 : Part 2 : 1985 Structural use of concrete : Part 2 Code of practice for special circumstances,
British Standards Institution
AC1319 : 1989 Building code requirements for reinforced concrete, American Concrete Institute
AS 3600 : 1988 Concrete structures, Standards Association of Australia
IS 456 : 2000
DIN 1045 July 1988 Structural use of concrete, design and construction, Deutsches Institut fur Normung E.V.
CEB-FIP Model code 1990, Comite Euro - International Du Belon
The composition of the technical committee responsible for the formulation of this standard is given in
For the purpose of deciding whether a particular requirement of this standard is complied with, the final value,
observed or calculated, expressing the result of a test or analysis shall be rounded off in accordance with
IS 2 : 1960 ‘Rules for rounding off numerical values (revised)‘. The number of significant places retained in the
rounded off value should be the same as that of~the specified value in this standard.
As in the Original Standard, this Page is Intentionally Left Blank
IS 456 : 2000
13.4 Construction Joints and Cold Joints
14.1 Work in Extreme Weather Conditions
14.2 Under-Water Concreting
15.2 Frequency of Sampling
15.3 Test Specimen
15.4 Test Results of Sample
SECTION 3 GENERAL DESIGN CONSIDERATION
18.1 Aim of Design
18.2 Methods of Design
18.3 Durability, Workmanship and Materials
18.4 Design Process
19.2 Dead Loads
19.3 Imposed Loads, Wind Loads and Snow Loads
19;4 Earthquake Forces
19.5 Shrinkage, Creep and Temperature Effects
19.6 Other Forces and Effects
19.7 Combination of Loads
19.8 Dead Load Counteracting Other Loads and Forces
19.9 Design Load
20.3 Probable Variation in Dead Load
20.4 Moment Connection
20.5 Lateral Sway
22.2 Effective Span
22.4 Structural Frames
22.5 Moment and Shear Coefficients for Continuous Beams
22.6 Critical Sections for Moment and Shear
22.7 Redistribution of Moments
23.0 Effective Depth
23.1 T-Beams and L-Beams
23.2 Control of Deflection
23.3 Slenderness Limits for Beams to Ensure Lateral Stability
24.2 Slabs Continuous Over Supports
24.3 Slabs Monolithic with Supports
24.4 Slabs Spanning in Two Directions~at Right Angles
24.5 Loads on Supporting Beams
25.2 Effective Length of Compression Members
25.3 Slenderness Limits for Columns
25.4 Minimum Eccentricity
26.2 Development of Stress in Reinforcement
26.3 Spacing of Reinforcement
26.4 Nominal Cover to Reinforcement
26.5 Requirements of Reinforcement for Structural Members
SECTION 4 SPECIAL DESIGN REQUIREMENTS FOR
STRUCTURAL MEMBERS AND SYSTEMS
29.2 Lever Arm
30.2 Analysis of Structure
IS 456 : 2000
30.5 Size and Position of Ribs
30.6 Hollow Blocks and Formers
30.7 Arrangement of Reinforcement
30.8 Precast Joists and Hollow Filler Blocks
3 1.1 General
31.3 Determination of Bending Moment
31.4 Direct Design Method
31.5 Equivalent Frame Method
31.6 Shear in Flat Slab
31.7 Slab Reinforcement
31.8 Openings in Flat Slabs
32.2 Empirical Design Method for Walls Subjected to Inplane Vertical Loads
32.3 Walls Subjected to Combined Horizontal and Vertical Forces
32.4 Design for Horizontal Shear
32.5 Minimum Requirements for Reinforcement in Walls
33.1 Effective Span of Stairs
33.2 Distribution of Loading on Stairs
33.3 Depth of Section
34.2 Moments and Forces
34.3 Tensile Reinforcement
34.4 Transfer of Load at the Base of Column
34.5 Nominal Reinforcement
SECTION 5 STRUCTURAL DESIGN (LIMIT STATE METHOD)
35 SAFETYAND SERVKEABlLITYkKNIREMl?N’l’s
35.2 Limit State of Collapse
35.3 Limit States of Serviceability
35.4 Other Limit States
36.1 Characteristic Strength of Materials
36.2 Characteristic Loads
36.3 Design Values
36.4 Partial Safety Factors
37.1 Analysis of Structure
38 LIMITSTATEOFCOLLAPSE :FLEXURE
39.2 Minimum Eccentricity
39.3 Short Axially Loaded Members in Compression
39.4 Compression Members with Helical Reinforcement
39.5 Members Subjected to Combined Axial Load and Uniaxial Bending
39.6 Members Subjected to Combined Axial Load and Biaxial Bending
39.7 Slender Compression Members
40 LLWTSTATEOF-COLLAPSE: SW
40.1 Nominal Shear Stress
40.2 Design Shear Strength of Concrete
40.3 Minimum Shear Reinforcement
40.4 Design of Shear Reinforcement
40.5 Enhanced Shear Strength of Sections Close to Supports
41 LJMITSTATEOFCOLLAPSE: TORSION
41.2 Critical Section
41.3 Shear and Torsion
41.4 Reinforcement in Members Subjected to Torsion
42.1 Flexural Members
LIST OF REFERRED INDIAN STANDARDS
STRUCTURAL DESIGN (WORKING STRESS METHOD)
B-l.1 General Design Requirements
B-1.2 Redistribution of Moments
B-l.3 Assumptions for Design of Members
B-2.1 Permissible Stresses in Concrete
B-2.2 Permissible Stresses in Steel Reinforcement
B-2.3 Increase in Permissible Stresses
B-3.1 Pedestals and Short Columns with Lateral ‘Des
B-3.2 Short Columns with Helical Reinforcement
B-3.3 Long Columns
B-3.4 Composite Columns
IS 456 : 2ooo
B-4 MYERS SUBJECTEDTOCOMBINEDAxw. LOADANDBENDING
Design Based on Untracked Section
Design Based on Cracked Section
Members Subjected to Combined Direct Load and Flexure
Nominal Shear Stress
Design Shear Strength of Concrete
Minimum Shear Reinforcement
Design of Shear Reinforcement
Enhanced Shear Strength of Sections Close to Supports
B-6.3 Shear and Torsion
B-6.4 Reinforcement in Members Subjected to Torsion
ANNEX C CALCULATION OF DEFLECTION
C-4 DE-ON DUETOCREEP
ANNEX D SLABS SPANNING IN TWO DIRECTIONS
ANNEX E EFFECTIVE LENGTH OF COLUMNS
ANNEX F CALCULATION OF CRACK WIDTH
ANNEX G MOMENTS OF RESISTANCE FOR RECTANGULAR AND T-SECTIONS
G- 1 RECTANGULARSECIIONS
G-1.1 Sections without CompressionReinforcement
G-1.2 Sections with Compression Reinforcement
ANNEX H COMMITTEE COMPOSITION
SECTION 1 GENERAL
k-1This standard deals with the general structural use
of plain and reinforced concrete.
1.1.1For the purpose of this standard, plain concrete
structures are those where reinforcement, if provided
is ignored for~determinationof strength of the structure.
1.2 Special requirements of structures, such as shells,
folded plates, arches, bridges, chimneys, blast resistant
structures, hydraulic structures, liquid retaining
structures and earthquake resistant structures, covered
in respective standards have not been covered in this
standard; these standards shall be used in conjunction
with this standard.
The Indian Standards listed in Annex A contain
provisions which through reference in this text,
constitute provisions of this standard. At the time of
publication, the editions indicated were valid. All
standards are subject to revision and parties to
agreements abasedon this standard are encouraged to
investigate the possibility of applying the most recent
editions of the standards indicated in Annex A.
3 TERMINOLOGY 1 -
For the purpose of this standard, the definitions given
in IS 4845 and IS 6461 (Parts 1 to 12) shall generally
For the purpose of this standard, the following letter
symbols shall have the meaning indicated againsteach,
where other symbols are used, they are explained at
the appropriate place:
Breadth of beam, or shorter dimension
of a rectangular column
Effective width of slab
Effective width of flange
Breadth of web or rib
Overall depth of beam or slab or
diameter of column; dimension of a
rectangular column in the direction
Thickness of flange
Effective depth of beam or slab
Depth of compression reinforcement
from the highly compressed face
ModuIus of elasticity of concrete
Modulusof elasticity of steel
characteristic cube compressive
strength of concrete
Modulus of rupture of concrete
(flexural tensile strength)
Splitting tensile strength of concrete
Characteristic strength of steel
Unsupported height of wall
Effective height of wall
Effective moment of inertia
Moment of inertia of the gross section
Moment of intertia of cracked section
Stiffness of member
Constant or coefficient or factor
Live load or imposed load
Horizontal distance between centres of
Length of a column or beam between
adequate lateral restraints or the
unsupported length of a column
Effective span of beam or slab or
effective length of column
Effective length about x-x axis
Effective length about y-y axis
Clear span, face-to-face of supports
I’,,for shorter of the two spans at right
Length of shorter side of slab
Length of longer side of slab
Distance between points of zero
moments in a beam
Span in the direction in which
moments are determined, centre to
centre of supports
Span transverse to I,, centre to centre
1z for the shorter of the continuous
Number of samples
Axial load on a compression member
Calculated maximum bearing pressure
IS 456 : 2000
Yc, - Calculated maximum bearing pressure
r - Radius
s - Spacing of stirrups or standard
T - Torsional moment
t - Wall thickness
V - Shear force
W - Total load
WL - Wind load
W - Distributed load per unit area
Wd - Distributed dead load per unit area
WI - Distributed imposed load per unit area
X - Depth of neutral axis
z - Modulus of section
Z - Lever arm
OZ,B - Angle or ratio
r, - Partial safety factor for load
xl - Partial safety factor for material
snl - Percentage reduction in moment
E -UC Creep strain of concrete
- Permissible stress in concrete in
OLX - Permissible stress in concrete in direct
Permissible stress in metal in direct
Permissible stress in steel in
Permissible stress in steel in tension
Permissible tensile stress in shear
Design bond stress
Shear stress in concrete
Maximum shear stress in concrete
with shear reinforcement
Nominal shear stress
Diameter of bar
SECTION 2 MATERIALS, WORKMANSHIP,
INSPECTION AND TESTING
The cement used shall be any of the following and the
type selected should be appropriate for the intended
33 Grade ordinary Portland cement
conforming to IS 269
43 Grade ordinary Portland cement
conforming to IS 8112
53 Grade ordinary Portland cement
conforming to IS 12269
Rapid hardening Portland cement conforming
to IS 8~041
Portland slag cement conforming to IS 455
Portland pozzolana cement (fly ash based)
conforming to IS 1489 (Part 1)
Portland pozzolana cement (calcined clay
based) conforming to IS 1489 (Part 2)
Hydrophobic cement conforming to IS 8043
Low heat Portland cement conforming to
Sulphate resisting Portland cement
conforming to IS 12330
Other combinations of Portland cement with mineral
admixtures (see 5.2) of quality conforming with
relevant Indian Standards laid down may also be used
in the manufacture of concrete provided that there are
satisfactory data on their suitability, such as
performance test on concrete containing them.
5.1.1 Low heat Portland cement conforming to
IS 12600 shall be used with adequate precautions with
regard to removal of formwork, etc.
5.1.2 High alumina cement conforming to IS 6452 or
supersulphated cement conforming to IS 6909 may be
used only under special circumstances with the prior
approval of the engineer-in-charge. Specialist literature
may be consulted for guidance regarding the use of
these types of cements.
5.1.3 The attention of the engineers-in-charge and
users of cement is drawn to the fact that quality of
various cements mentioned in 5.1 is to be determined
on the basis of its conformity to the performance
characteristics given in the respective Indian Standard
Specification for thatcement. Any trade-mark or any
trade name indicating any special features not covered
in the standard or any qualification or other special
performance characteristics sometimes claimed/
indicated on the bags or containers or in advertisements
alongside the ‘Statutory Quality Marking’ or otherwise
have no relation whatsoever with the characteristics
guaranteed by the Quality Marking as relevant to that
cement. Consumers are, therefore, advised to go by
the characteristics as given in the corresponding
Indian Standard Specification or seek specialist
advise to avoid any problem in concrete making and
5.2 Mineral Admiitures
Pozzolanic materials conforming to relevant Indian
Standards may be used with the permission of the
engineer-in-charge, provided uniform blending with
cement is ensured.
22.214.171.124 Fly ash (pulverizedfuel ash)
FIy ash conforming to Grade 1 of IS 3812 may be
use?,as part replacement of ordinary Portland cement
provided uniform blending with cement is ensured.
Silica fume conforming to a standard approved by the
deciding authority may be used as part replacement of
cement provided uniform blending with the cement is
NOTE-The silica fume (very fine non-crystalline silicon
dioxide)is aby-productofthemanufactmeof silicon,kmxilicon
orthe like, fromquartzandcarbonin electricarcfurnace.It is
of a mix.
126.96.36.199Rice husk ash
Rice husk ash giving required performance and
uniformity characteristics -may be used with the
approval of the deciding authority.
NOTE--Rice husk ash is producedby burningrice husk and
containlargepropotion of silica. To achieve amorphousstate,
ricehuskmaybe burntatcontrolledtemperatum.Itis necessary
and uniformitysince it can rangefrombeing as dekterious as
silt when incorporatedin concmte. Waterdemnndand drying
&i&age shouldbe studiedbeforeusing ria husk.
Metakaoline having fineness between 700 to
900 m?/kg may be used as ~pozzolanic material in
NOTE-Metaknoline is obtained by calcination of pun or
followed by grind& to achieve a A of 700 to 900 n?/kg.
Theresultingmaterialhas high pozzolanicity.
5.2.2 Ground Granulated Blast Furnace Slag
Ground granulated blast furnace slag obtained by
grinding granulated blast furnace slag conforming to
IS 12089may be used as part replacement of ordinary
IS 456 : 2000
Portland cements provided uniform blending with
cement is ensured.
Aggregates shall comply with the requirements of
IS 383. As far as possible preference shall be given to
5.3.1 Other types of aggregates such as slag and
crushed overbumt brick or tile, which may be found
suitable with regard to strength, durability of concrete
and freedom from harmful effects may be usedfor plain
concrete members, but such aggregates should not
contain more than 0.5 percent of sulphates as SO, and
should not absorb more than 10 percent of their own
mass of water.
5.3.2 Heavy weight aggregates or light weight
aggregates such as bloated clay aggregates and sintered
fly ash aggregates may also be used provided the
engineer-in-charge is satisfied with the data on the
properties of concrete made with them.
NOTE-Some of the provisions of the code would require
may be consultedfor guidance.
5.3.3 Size of Aggregate
The nominal maximum size of coarse aggregate should
be as large as possible within the limits specified but
in no case greater than one-fourth of the minimum
thickness of the member, provided that the concrete
can be placed without difficulty so as to surround all
reinforcement thoroughly and fill the comers of the
form. For most work, 20 mm aggregate is suitable.
Where there is no restriction to the flow of concrete
into sections, 40 mm or larger size may be permitted.
In concrete elements with thin sections, closely spaced
reinforcement or small cover, consideration should be
given to the use of 10 mm nominal maximum size.
Plums above 160 mm and up to any reasonable size
may be used in plain concrete work up to a maximum
limit of 20 percent by volume of concrete when
specifically permitted by the engineer-in-charge. The
plums shall be distributed evenly and shallbe not closer
than 150 mm from the surface.
188.8.131.52 For heavily reinforced concrete members as
in the case of ribs of main beams, the nominal
maximum size of the aggregate should usually be
restricted to 5 mm less than the minimum clear distance
between the main bars or 5 mm less than the minimum
cover to the reinforcement whichever is smaller.
5.3.4 Coarse and fine aggregate shall be batched
separately. All-in-aggregate may be used only where
specifically permitted by the engineer-in-charge.
Water used for mixing and curing shall be clean and
free from injurious amounts of oils, acids, alkalis, salts,
sugar, organic materials or other substances that may
be deleterious to concrete or steel.
Potable water is generally considered satisfactory
for mixing concrete. As a guide the following
concentrations represent the maximum permissible
To neutralize 100 ml sample of water, using
phenolphthalein as anindicator, it should not
require more than 5 ml of 0.02 normal NaOH.
The details of test are given in 8.1 of IS
3025 (Part 22).
To neutralize 100 ml sample of water, using
mixed indicator, it should not require more
than 25 ml of 0.02 normal H$O,. The details
of ‘test shall be as given in 8 of IS 3025
Permissible limits for solids shall be as given
in Table 1.
In case of doubt regarding development of
strength, the suitability of water for making concrete
shall be ascertained by the compressive strength and
initial setting time tests specified in 184.108.40.206 and 220.127.116.11.
18.104.22.168 The sample of water taken for testing shall
represent the water proposed to be used for concreting,
due account being paid to seasonal variation. The
sample shall not receive any treatment before testing
other than that envisaged in the regular supply of water
proposed for use in concrete. The sample shall be stored
in a clean container previously rinsed out with similar
S.4.1.2 Average 28 days compressive strength of at
least three 150mm concrete cubes prepared with water
proposed to be used shall not be less than 90 percent
of the average of strength of three similar concrete
cubes prepared with distilled water. The cubes shall
be prepared, curedand tested in accordance with the
requirements of IS 516.
22.214.171.124 The initial setting time of test block made with
theappropriate cement and the water proposed to be
used shall not be less than 30 min and shall not differ
by& 30min from the initial setting time of control
test block prepared with the same cement and distilled
water. The test blocks shall be preparedand tested in
accordance with the requirements off S 4031 (Part 5).
5.4.2 The pH value of water shall be not less than 6.
5.4.3 Sea Water
Mixing or curing of concrete with sea water is not
recommended because of presence of harmful salts in
sea water. Under unavoidable circumstances sea water
may be used for mixing or curing in plain concrete with
no embedded steel after having given due consideration
to possibledisadvantagesandprecautions including use
of appropriate cement system.
‘lhble 1 Permissible Limit for !Wids
SI -apu Permb?dbleLImlt,
i) organic IS 3a25 (Pal-l18) 2(Jomgll
ii) Inorganic IS 3025 (yalt 18) 3ooomo/L
iii) Sulphaki (usSOJ IS302s(Part24) amo/l
iv) Chlorides(as Cl) IS 3025 (part32) 2ooompll
forfxmaetc not Containing
forleInfolced collcntc worlr
v) Suspfmdedmatter IS 3025 (Palt17) 2(xJom%l
5.4.4 Water found satisfactory for mixing is also 5.6.1 All reinforcement shall be free from loose mill
suitable for curing concrete. However, water used for scales, loose rust and coats of paints, oil, mud or any
curing should not produce any objectionable stain or other substances which may destroy or reduce bond.
unsightly deposit on the concrete surface. The presence Sand blasting or other treatment is recommended to
of tannic acid or iron compounds is objectionable. clean reinforcement.
5.5.1 Admixture, if used shall comply with IS 9103.
Previous experience with and data on such materials
shouldbe considered in relationto thelikely standa& of
55.2 Admixtures should not impair durability of
concrete nor combine with the constituent to form
harmful compounds nor increase the risk of corrosion
5.6.2 Special precautions like coating of reinforcement
may be required for reinforced concrete elements in
exceptional cases and for~rehabilitation of structutes.
Specialist literature may be referred to in such cases.
5.6.3 The modulus of elasticity of steel shall be taken
as 200 kN/mm*. The characteristic yield strength of
different steel shall be assumed as the minimum yield
stress/O.2percent proof stress specified in the relevant
55.3 The workability, compressive strength and the
slump loss of concrete with and without the use of
admixtures shall be established during the trial mixes
before use of admixtures.
5.7 Storage of Materials
Storage of materials shall be as described in IS 4082.
5.5.4 The relative density of liquid admixtures shall
be checked for each drum containing admixtures and
compared with the specified value before acceptance.
5.5.5 The chloride content of admixtures shall
be independently tested for each batch before
The concrete shall be in grades designated as per
6.1.1 The characteristic strength is defined as the
strength of material below which not more than
5 percent of the test results are expectedto fall.
5.5.6 If two or more admixtures are used
simultaneously in the same concrete mix, data should
be obtained to assess their interaction and to ensure
The reinforcement shall be any of the following:
6.1.2 The minimum grade of concrete for plain and
reinforced concrete shall be as per Table 5.
61.3 Concrete of grades lower than those given in
Table-5 may be used for plain concrete constructions,
lean concrete, simple foundations, foundation for
masonry walls and other simple or temporary
reinforced concrete construction.
Mild steel and medium tensile steel bars
conforming to IS 432 (Part 1).
High strength deformed steel barsconforming
to IS 1786.
6.2 Properties of Concrete
63.1 Increase of Strength with Age
Hard-drawn steel wire fabric conforming to
Structural steel conforming to Grade A of
There is normally a gain of strength beyond 28 days.
The quantum of increase depends upon the gradeand
type of cement, curing and environmental conditions,
etc. The design should be based on 28 days charac-
teristic strengthof concrete unless there is a evidence to
IS 456 : 2000
Table 2 Grades cifConcrete
(Clau.re6.1,9.2.2, 15.1.1 and36.1)
Group Grade Designation SpecifiedCharacte~tk
150 mm Cube at 28 Days in
(1) (2) (3)
Ordinary M 10 10
Concrete M 15 15
M 20 20
Standard M 25 25
Concrete M 30 30
M 35 35
M 45 45
M JO 50
M 55 55
High M60 60
Strength M65 65
Concrete M70 70
M 80 80
1 Inthedesignationof concretemix Mmfm to themix andthe
numberto the specified compressivestrengthof 150 mm size
cube at28 days, expressedin N/mn?.
2 Forconcreteof compressivestrengthgreata thanM 55,design
parametersgiven in the stand& may not be applicableandthe
values may be obtoined from specialized literatures and
justify a higher strength for a particular structure due to
126.96.36.199 For concrete of grade M 30 and above, the
rate of increase of compressive strength with age shall
be based on actual investigations.
188.8.131.52 Where members are subjected to lower direct
load during construction, they should be checked for
stresses resulting from combination of direct load and
bending during construction.
6.2.2 Tensile Strength of Concrete
The flexural and splitting tensile strengths shall be
obtained as described in IS 516 and IS 5816
respectively. When the designer wishes to use an
estimate of the tensile strength from the compressive
strength, the following formula may be used:
Flexural strength, f, = 0.7.& N/mm2
wheref&is the characteristic cube compressive strength
of concrete in N/mmz.
6.2.3 Elastic Deformation
The modulus of elasticity is primarily influenced by
the elastic properties of the aggregate and to a lesser
extent by the conditions of curing qd age of the
concrete, the mix proportions and the type of cement.
The modulus of elasticity is normally related to the
compressive strength of concrete.
184.108.40.206 The modulus of elasticity of concrete can be
assumed as follows:
E, is the short term static modulus of elasticity in
Actual measured values may differ by f 20 percent
from the values dbtained from the above expression.
The total shrinkage of concrete depends upon the
constituents of concrete, size of the member and
environmental conditions. For a given humidity and
temperature, the total shrinkage of concrete is most
influenced by the total amount of water present in the
concrete at the time of mixing and, to a lesser extent,
by the cement content.
220.127.116.11 In the absence of test data, the approximate
value of the total shrinkage strain for design may be
taken as 0.000 3 (for more information, see-IS 1343).
6.2.5 Cmep of Concrete
Creep of concrete depends,in addition to the factors
listed in 6.2.4, on the stress in the concrete, age at
loading and the duration of loading. As long as the
stress in concrete does not exceed one-third of its
characteristic compressive strength, creep may be
assumed to be proportional to the stress.
6.25.11n the absence of experimental data and detailed
information on the effect of the variables, the ultimate
creep strain may be estimated from the following
valuesof creep coefficient (that is, ultimatecreep strain/
elastic strain at the age of loading); for long span
structure, it is advisable to determine actual creep
strain, likely to take place:
Age at Loading Creep Coeficient
7 days 2.2
28 days 1.6
does not includethe elastic strain.
6.2.6 Thermal Expansion
The coefficient df thermal expansion depends on nature
of cement, the aggregate, the cement content, the
relative humidity and the size of sections-The value
of coefficient of thermal expansion for concrete with
different aggregates may be taken as below:
npe of Aggregate
Coeficient of Thermal
1.2 to 1.3 x 10-S
0.9 to 1.2 x 1cP
0.7 to 0.95 x 10-J
O.%to 0.95 x lo5
0.6 t@.9 x 10s
IS 456 : 2000
7 WORKABILITY OF CONCRETE
7.1 The concrete mix proportions chosen should be be compacted with the means available. Suggested
such that the concrete is of adequate workability for ranges of workability of concrete measured in
the placing conditions of the concrete and can properly accordance with IS 1199 are given below:
Placing Conditions Degree of Slump
(1) (2) (3)
Blinding concrete; Very low See 7.1.1
Pavements using pavers I
sections in slabs,
beams, walls, columns;
Hand placed pavements;
MediumHeavily reinforced 50-100
sections in slabs,
beams, walls, columns; 75-100
Pumped concrete 1
Trench fill; High 100-150
Tremie concrete I Very high See 7.1.2
NOTE-For most of the placing conditions, internal vibrators (needle vibrators) are suitable. The diameter of tbe needle shall be
determined based on the density and spacing of reinforcement bars and thickness of sections. For tremie concrete, vibrators am not
rewired to be used (see &SO13.3).
7.1.1 In the ‘very low’ category of workability where
strict control is necessary, for example pavement
quality concrete, measurement of workability by
determination of compacting factor will be more
appropriate than slump (see IS 1199) and a value of
compacting factor of 0.75 to 0.80 is suggested.
7.1.2 In the ‘very high’ category of workability,
measurement of workability by determination of flow
will be appropriate (see IS 9103).
8 DURABILITY OF CONCRETE
A durable concrete is one that performs satisfactorily
in the working environment during its anticipated
exposure conditions during service. The materials and
mix proportions specified and used should be such as
to maintain its integrity and, if applicable, to protect
embedded metal from corrosion.
8.1.1 One of the main characteristics influencing the
durability of concrete is its permeability to the ingress
of water,oxygen, carbon dioxide, chloride, sulphateand
is governed by the constituents and workmanship used
in making the concrete. with normal-weight aggregates
a suitably low permeability is achieved by having an
adequate cement content, sufficiently low free water/
cement~ratio,~byensuring complete compaction of the
concrete, and by adequate curing.
The factors influencing durability include:
the cover to embedded steel;
the typeand_quality of constituent materials;
the cement content and water/cement ratio of
workmanship, to obtain full compaction and
efficient curing; and
the shape and size of the member.
The degree of exposure anticipated for the concrete
during its service life together with other relevant
factors relating to mix composition, workmanship,
design and detailing should be considered. The
concrete mix to provide adequate durability under these
conditions should be chosen taking account of the
accuracy of current testing regimes for control and
compliance as described in this standard.
IS 456 : 2000
8.2 Requirements for Durability
8.2.1 Shape and Size of Member
The shape or design details of exposed structures
should be such as to promote good drainage of water
and to avoid standing pools and rundown of water.
Care should also be taken to minimize any cracks that
may collect or transmit water. Adequate curing is
essential to avoid the harmful effects of early loss of
moisture (see 13S).Member profiles and their
intersections with other members shall be designed and
detailed in a way to ensure easy flow of concrete and
proper compaction during concreting.
Concrete is more vulnerable to deterioration due to
chemical or climatic attack when it is in thin sections,
in sections under hydrostatic pressure from one side
only, in partially immersed sections and at corners and
edges of elements. The life of the strycture can be
lengthened by providing extra cover to steel, by
chamfering the corners or by using circular cross-
sections or by using surface coatings which prevent or
reduce the ingress of water, carbon dioxide or
8.2.2 Exposure Conditions
18.104.22.168 General environment
The general environment tc, which the concrete will
be exposed during its working life is classified into
five levels of severity, that is, mild, moderate, severe,
very severe and extreme as described in Table 3.
Table 3 Environmental Exposure Conditions
(Chwes 22.214.171.124 and 35.3.2)
Sl No. Environment
Nominal Maximum Size Entrained Air
Since air entrainment reduces the strength, suitable
adjustments may be made in the mix design for
achieving required strength.
126.96.36.199 Exposure to sulphate attack
Table 4 gives recommendations for the type of cement,
maximum free water/cement ratio and minimum
cement content, which arerequired atdifferent sulphate
concentrations in near-neutral ground water having
Concrete surfaces protected against
those situatedin coastalarea.
Concrete surfaces sheltered from
saturatedsalt airin coastalarea
Concrete surfaces exposed to severe
rain, alternate wetting and drying or
occasional freezingwhilst wet orsevere
For the very high sulphate concentrations in Class 5
conditions, some form of lining such as polyethylene
or polychloroprene sheet; or surface coating based on
asphalt, chlorinated rubber, epoxy; or polyurethane
materials should also be used to prevent access by the
8.2.3 Requirement of Concrete Cover
188.8.131.52 The protection of the steel in concrete against
corrosion depends upon an adequate thickness of good
184.108.40.206 The nominal cover to the reinforcement shall
be provided as per 26.4.
Concretesurfacesexposed to sea water
conditions whilst wet
Concrete in contact with or buried
Surfaceof membersin tidalzone
Membersin direct contact with liquid/
Specialist literatures may be referred to for durability
requirementsof concrete surfaces exposed to abrasive
action,for example,incaseof machineryandmetaltyres.
220.127.116.11 Freezing and thawing
Where freezing and thawing actions under wet
conditions exist, enhanced durability can be obtained
by the use of suitable air entraining admixtures. When
concrete lower than grade M 50 is used under these
conditions, the mean total air content by volume of
the fresh concrete at the time df delivery into the
construction should be:
0.2.4 Concrete Mix Proportions
The free water-cement ratio is an important factor in
governing the durability of concrete and should always
be the lowest value. Appropriate values for minimum
cement content and the maximum free water-cement
ratio are given in Table 5 for different exposure
conditions. The minimum cement content and
maximum water-cement ratio apply to 20 mm nominal
maximum size aggregate. For other sizes of aggregate
they should be changed as given in Table 6.
IS 456 : 2000
18.104.22.168 Maximum cement content been given in design to the increased risk of cracking
Cement content not including fly ash and ground due to drying shrinkage in.thin sections, or to early
granulated blast furnace slag in excess of 450 kg/x$ thermal cracking and to the increased risk of damage
should not be used unless special consideration has due to alkali silica reactions.
Table 4 Requirements for Concrete Exposed to Sulphate Attack
(Clauses 22.214.171.124 and 9.1.2)
ChSS Concentration ofSulphates,
Expressed a~ SO,
Total SO, SO,in In Ground
2:l water: Water
(1) (2) (3)
0 1 TraCeS
ii) 2 0.2 to
iii) 3 0.5 to
Less than LesSthan
iv) 4 1.0to 3.1 to
v) 5 More than More than
Type ofCement Dense, Fully Compacted concrete.
Made with 20 mm Nominal
Maximum Size Aggregates
Complying with IS 383
cement or Portland
slag cement or
cement or Podand
Portland cement or
with protective coatings
1 Cement content given in this table is irrespective of grades of cement.
2 Use of supersulphated cement is generally restricted where the prevailing temperature is above 40 “c.
3 Supersulphated cement gives~anacceptable life provided that the concrete is dense and prepared with a water-cement mtio of 0.4 or
less, in mineral acids, down to pH 3.5.
4 The cement contents given in co16 of this table are the minimum recommended. For SO, contents near tbe upper limit of any class,
cement contents above these minimum are advised.
5 For severe conditions, such as thin sections under hydrostatic pressure on one side only and sections partly immersed, considerations
should be given to a further reduction of water-cement ratio.
6 Portland slag cement conforming to IS 455 with slag content more than 50 percent exhibits better sulphate resisting properties.
7 Where chloride is encountered along with sulphates in soil or ground water, ordinary Portland cement with C,A content from 5 to 8
percent shall be desirable to be used in concrete, instead of sulphate resisting cement. Alternatively, Portland slag cement conforming
to IS 455 having more than 50percent slag or a blend of ordinary Portland cement andslag may be used provided sufficient information
is available on performance of such blended cements in these conditions.
IS 456 : 2000
8.2.5 Mix Constituents
For concrete to be durable, careful selection of the mix
and materials is necessary, so that deleterious
constituents do not exceed the limits.
126.96.36.199 Chlorides in concrete
Whenever there is chloride in concrete there is an
increased risk of corrosion of embedded metal. The
higher the chloride content, or if subsequently exposed
to warm moist conditions, the greater the risk of
corrosion. All constituents may contain chlorides and
concrete may be contaminated by chlorides from the
external environment. To minimize the chances of
deterioration of concrete from harmful chemical salts,
the levels of such harmful salts in concrete coming
from concrete materials, that is, cement, aggregates
water and admixtures, as well as by diffusion from the
environment should be limited. The total amount of
chloride content (as Cl) in the concrete at the time of
placing shall be as given in Table 7.
The total acid soluble chloride content should be
calculated from the mix proportions and the measured
chloride contents of each of the constituents. Wherever
possible, the total chloride content of the concrete
should be determined.
188.8.131.52 Sulphates in concrete
Sulphates are present in most cements and in some
aggregates; excessive amounts of water-soluble
sulphate from these or other mix constituents can cause
expansion and disruption of concrete. To prevent this,
the total water-soluble sulphate content of the concrete
mix, expressed as SO,, should not exceed 4 percent by
mass of the cement in the mix. The sulphate content
should be calculated as the total from the various
constituents of the mix.
The 4 percent limit does not apply to concrete made
with supersulphated cement complying with IS 6909.
184.108.40.206 Alkali-aggregate reaction
Some aggregates containing particular varieties of
silica may be susceptible to attack by alkalis (N%O
and %O) originating from cement or other sources,
producing an expansive reaction which can cause
cracking and disruption of concrete. Damage to
concrete from this reaction will normally only occur
when .a11the following are present together:
a) A high moisture level, within the concrete;
b) A cement with high alkali content, or another
source of alkali;
c) Aggregate containing an alkali reactive
Where the service records of particular cement/
aggregate combination are well established, and do not -
include any instances of cracking due to alkali-
aggregate reaction, no further precautions should be
necessary. When the materials are unfamiliar,
precautions should take one or more of the following
a) Use of non-reactive aggregate from alternate
Table 5 Minimum CementContent, Maximum Water-Cement Ratio and Minimum Grade of Concrete
for Different Exposures with Normal Weight Aggregates of 20 mm Nominal Maximum Size
(Clauses 6.1.2, 220.127.116.11 and9.1.2)
Exposure Plain Concrete Reinforced Concrete
/ - * -
Minimum Maximum Minimum Minimum Maximum Minimum
Cement Free Water- Grade of Cement Free Water- Grade of
Content Cement Ratio Concrete’ Content Cement Ratio Concrete
(2) (3) (4) (5) (6) (7) 0-9
Mild 220 0.60 300 0.55 M 20
Moderate 240 0.60 M 15 300 0.50 M 25
Severe 250 0.50 M 20 ~320 0.45 M 30
Very severe 260 0.45 M 20 340 0.45) M 35
Extreme 280 0.40 M25 360 0.40 M40
1 Cement content prescribed in this table is irrespective of the grades of cement and it is inclusive of ad&ons mentioned in 5.2. The
additions such as fly ash or ground granulated blast furnace slag may be taken into account in the concrete composition with respect to
Ihe cement content and water-cement ratio if the suitability is established and as long as the maximum amounts taken into account do
not exceed the limit of pozzolona and slag specified in IS 1489(Part I) and IS 455 respectively.
2 Minimum gradefor plain concrete under mild exposure condition is not specified.
Table 6 Adjustments to Minimum Cement
Contents for Aggregates Other Than 20 mm
Nominal Maximum Size
Sl Nominal Maximum Adjustmenk to Minimum Cement
No. Aggregate Size Contents in Table 5
(1) (2) (3)
i) 10 +40
ii) 20 0
iii) 40 -30
Tabie 7 Limits of Chloride Content of Concrete
Type or Use of Concrete Maximum Total
Expressed as k&n’ of
Concrete containingmetaland 0.4
Reinforcedconctite or plainconcrete 0.6
Concretenot containingembedded 3.0
metal orany materialquiring
Use of low alkali ordinary ‘Portland cement
having total alkali content not more than 0.6
Further advantage can be obtained by use of fly
ash (Grade 1) conforming to IS 3812 or
granulated blastfurnace slag conforming to
IS 12089 as part replacement of ordinary
Portland cement (having total alkali content as
Na,O equivalent not more than 0.6 percent),
provided fly ash content is at least 20 percent
or slag content is at least 50 percent.
Measures to reduce the degree of saturation of
the concrete during service such as use of
Limitingthe cement content in the concrete mix
and thereby limiting total alkali content in the
concrete mix. For more guidance specialist
literatures may be referred.
8.2.6 Concrete in Aggressive Soils and Water
The destructive action of aggressive waters on concrete
is progressive. The rate of deterioration decreases as
the concrete~ismade stronger and more impermeable,
and increases as the salt content of the water increases.
Where structures are only partially immersed or are in
contact with aggressive soils or waters on one side only,
evaporation may cause serious concentrations of salts
with subsequent deterioration, even where the original
salt content of the soil or water is not high.
to sulphatenttackis given in 18.104.22.168.
At sites where alkali concentrations are high or may
become very high, the ground water should be lowered
by drainageso that it will not come into direct contact
with the concrete.
Additional protection may be obtained by the use of
chemically resistant stone facing or a layer of plaster
of Paris covered with suitable fabric, such as jute
thoroughly impregnated with bituminous material.
8.2.7 Compaction, Finishing and Curing
Adequate compaction without segregation should be
ensured by providing suitable workability and by
employing appropriate placing and compacting
equipment and procedures. Full compaction is
particularly important in the vicinity of construction
and movement joints and of embedded water bars and
Good finishing practices are essential for durable
Overworking the surface and the addition of water/
cement to aid in finishing should be avoided; the
resulting laitance will have impaired strength and
durability and will be particularly vulnerable to
freezing and thawing under wet conditions.
It is essential to use proper and adequate curing
techniques to reduce the permeability of the concrete
and enhance its durability by extending the hydration
of the cement, particularly in its surface zone
8.2.8 Concrete in Sea-water
Concrete in sea-water or exposed directly along the
sea-coast shall be at least M 20 Grade in the case of
plain concrete andM 30 in case of reinforced concrete.
The use of slag or pozzolana cement~isadvantageous
under such conditions.
22.214.171.124 Special attention shall be.given to the design
of the mix to obtain the densest possible concrete; slag,
broken brick, soft limestone, soft sandstone, or other
porous or weak aggregates shall not be used.
126.96.36.199 As far as possible, preference shall be given to
precast members unreinforced, well-cured and
hardened, without sharp comers, and having trowel-
smooth finished surfaces free from crazing, cracks or
other defects; plastering should be avoided.
188.8.131.52 No construction joints shall be allowed within
600 mm below low water-level or within 600 mm of
the upper and lower planes of wave action. Where
IS 456 : 2000
unusually severe conditions or abrasion’areanticipated,
such parts of the work shall be protected by bituminous
or silica-fluoride coatings or stone facing bedded with
184.108.40.206 In reinforced concrete structures, care shall be
taken to protect the reinforcement from exposure to
saline atmosphere during storage, fabrication and use.
It may be achieved by treating the surface of
reinforcement with cement wash or by suitable
9 CONCRETE MIX PROPORTIONING
9.1 Mix Proportion
The mix proportions shall be selected to ensure the
workability of the fresh concrete and when concrete is
hardened, it shall have the required strength, durability
and surface finish.
9.1.1 The determination of the proportions of cement,
aggregates and water to attain the required strengths
shall be made as follows:
a) By designing the concrete mix; such concrete
shall be called ‘Design mix concrete’, or
b) By adopting nominal concrete mix; such
concrete shall be called ‘Nominalmix concrete’.
Design mix concrete is preferred to nominal mix. If
design mix concrete cannot be used for any reason on
the work for grades of M 20 or lower, nominal mixes
may be used with the permission of engineer-in-charge,
which, however, is likely to involve a higher cement
9.1.2 Information Required
In specifying a particular grade of concrete, the
following information shall be included:
Type of mix, that is, design mix concrete or
nominal mix concrete;
Type of cement;
Maximum nominal size of aggregate;
Minimum cement content (for design mix
Maximum water-cement ratio;
Mix proportion (for nominal mix concrete);
Exposure conditions as per Tables 4 and 5;
Maximum temperature of concrete at the time
m>Method of placing; and
n>Degree of supervision.
220.127.116.11 In appropriate circumstances, the following
additional information may be specified:
Maximum cement content, and
Whether an admixture shall or shall not be
used and the type of admixture and the
condition of use.
9.2 Design Mix Concrete
9.2.1 As the guarantor of quality of concrete used in
the construction, the constructor shall carry out the mix
design and the mix so designed (not the method of
design) shall be approved by the employer within the
limitations of parameters and other stipulations laid
down by this standard.
9.2.2 The mix shall be designed to produce the grade
of concrete having the required workability and a
characteristic strength not less than appropriate values
given in Table 2. The target mean strength of concrete
mix should be equal to the characteristic strength plus
1.65 times the standard deviation.
9.2.3 Mix design done earlier not prior to one year
may be considered adequate for later work provided
there is no change in source and the quality of the
9.2.4 Standard Deviation
The standarddeviation for each grade of concrete shall
be calculated, separately.
18.104.22.168 Standard deviation based on test strength of
Number of test results of samples-The total
number of test strength of samples required to
constitute an acceptable record for calculation
of standard deviation shall be not less than 30.
Attempts should be made to obtain the 30
samples, as early as possible, when a mix is used
for the first time.
In case of si&icant changes in concrete-
When significant changes are made in the
production of concrete batches (for example
changes in the materials used, mix design.
equipment Drtechnical control), the standard
deviation value shall be separately calculated
for such batches of concrete.
Standard deviation to be btvught up to date-
The calculation of the standard deviation shall
be brought up to date after every change of mix
22.214.171.124 Assumed stanaianldeviation
Where sufficient test results for a particular grade of
concrete are not available, the value of standard
deviation given in Table 8 may be assumed for design
of mix in the first instance. As soon as the results of
samples are available, actual calculated standard
deviation shall be used and the mix designed properly.
However, when adequatepast mcordsfor a similargrade
d&rent fromthatshowninTable 8,itshallbepem&ible
Table 8 Assumed Standard Deviation
(Clause 126.96.36.199 and Table 11)
M40 1 5.0
NOTE-The above values correspondto the site contrdihaving
properstorageof cement;weigh batchingof allmaterials;controlled
addition of ~water;regular checking of all matials. aggregate
gradings and moisture content; and periodical checking of
workability and strength.Wherethereis deviationfromthe above
the values given in the above tableshall be increasedby lN/inm*.
9.3 Nominal Mix Concrete
Nominal mix concrete may be used for concrete of
M 20 or lower. The proportions of materials for
nominal mix concrete shall be in accordance with
9.3.1 The cement content of the mix specified in
Table 9 for any nominal mix shall be proportionately
increased if the quantity of water in a mix has to be
increase&o overcome the difficulties of placement and
compaction, so that the water-cement ratio as specified
is not exceeded.
IS 456 : 2000
10 PRODUCTION OF CONCRETE
10.1 Quality Assurance Measures
10.1.1 In order that the properties of the completed
structure be consistent with the requirements and the
assumptions made during the planning and the design,
adequate quality assurance measures shall be taken.
The construction should result in satisfactory strength,
serviceability and long term durability so as to lower
the overall life-cycle cost. Quality assurance in
construction activity relates to proper design, use of
adequate materials and components to be supplied by
the producers, proper workmanship in the execution
of works by the contractor and ultimately proper care
during the use of structure including timely
maintenance and repair by the owner.
10.1.2 Quality assurance measures are both technical
and organizational. Some common cases should be
specified in a general Quality Assurance Plan which
shall identify the key elements necessary to provide
fitness of the structure and the means by which they
are to be provided and measured with the overall
purpose to provide confidence that the realized project
will work satisfactorily in service fulfilling intended
needs. Thejob of quality control and quality assurance
would involve quality audit of both the inputs as well
as the outputs. Inputs are in the form of materials for
concrete; workmanship in all stages of batching,
mixing, transportation, placing, compaction and
curing; and the related plant, machinery and
equipments; resulting in the output in the form of
concrete in place. To ensure proper performance, it is
necessary that each step in concreting which will be
covered by the next step is inspected as the work
proceeds (see also 17).
Table 9 Proportions for Nominal Mix-Concrete
(Clauses9.3 and 9.3.1)
Total Qua&y of Dry Aggre-
gates by hhc-per SOkg of
Cement, to be Taken at?the Sum
of the Individual Masses of
F’lneand Coarse Aggregates, kg,
Proportion of Fine Quantity of Water per
&gregate to Coarse 50 kg of Cement, Mar
Aggregate (by Mad 1
(1) (2) (3) (4)
M 7.5 625 anupperlimitof 1:1*/sanda 45
M 10 480 lowerlit of 1:2V, 34
M 15 330 32
M20 250 30
NOTE-The proportionof the fine to coarseaggmgatesshouldbe adjustedfromupperlimitto lowerlimit~progressivelyas the grading
of fine aggregatesbecomes finerandthe maximumsize of coarseaggregatebecomes larger.Gradedcoarseaggregateshall be used.
For an averagegradingof tine aggregate(thatis. Zone II of Table4 of IS 383). the proportionsshall be 1:1I/,, I:2 and 1:2’/, for
maximumsize of aggregates10mm, 20 mm and40 mmrespectively.
IS 456 :2000
10.1.3 Each party involved in the realization of a
project should establish and implement a Quality
Assurance Plan, for its participation in the project.
Supplier’s and subcontractor’s activities shall be
covered in the plan. The individual Quality Assurance
Plans shall fit into the general Quality Assurance Plan.
A Quality Assurance Plan shall define the tasks and
responsibilities of all persons involved, adequate
control and checking procedures, and the organization
and maintaining adequate documentation of the
building process and its results. Such documentation
should generally include:
test reports and manufacturer’s certificate for
materials, concrete mix design details;
pour cards for site organization and clearance
for concrete placement;
record of site inspection of workmanship, field
non-conformance reports, change orders;
quality control charts; and
NOTE-Quality control charts are recommended wherever the
concrete is in continuous production over considerable period.
To avoid confusion and error in batching, consideration
should be given to using the smallest practical number
of different concrete mixes on any site or in any one
plant. In batching concrete, the quantity of both cement
and aggregate shall be determined by mass; admixture,
if solid, by mass; liquid admixture may however be
measured in volume or mass; water shall be weighed
or measured by volume in a calibrated tank (see also
Ready-mixed concrete supplied by ready-mixed
concrete plant shall be preferred. For large and medium
project sites the concrete shall be sourced from ready-
mixed concrete plants or from on site or off site
batching and mixing plants (see IS 4926).
10.2.1 Except where it can be shown to the satisfaction
of the engineer-in-charge that supply of properly
graded aggregate of uniform quality can be maintained
over a period of work, the grading of aggregate should
. be controlled by obtaining the coarse aggregate in
different sizes and blending them in the right
proportions when required, the different sizes being
stocked in separate stock-piles. The material should
be stock-piled for several hours preferably a day before
use. The grading of coarse and fine aggregate should
be checked as frequently as possible, the frequency
for a given job being determined by the engineer-in-
charge to ensure that the specified grading is
10.2.2 The accuracy of the measuring equipment shall
Abewithin + 2 percent of the quantity of cement being
measured and within + 3 percent of the quantity of
aggregate, admixtures and water being measured.
10.2.3 Proportion/Type and grading of aggregates shall
be made by trial in such a way so as to obtain densest
possible concrete. All ingredients of the concrete
should be used by mass only.
10.2.4 Volume batching may be allowed only where
weigh-batching is not practical and provided accurate
bulk densities of materials to be actually-used in
concrete have earlier been established. Allowance for
bulking shall be made in accordance with IS 2386
(Part 3). The mass volume relationship should be
checked as frequently as necessary, the frequency for
the given job being determined by engineer-in-charge
to ensure that the specified grading is maintained.
N2.5 It is important to maintain the water-cement
ratio constant at its correct value. To this end, determi-
nation of moisture contents in both fine and coarse
aggregates shall be made as frequently as possible, the
frequency for a given job being determined by the
engineer-in-charge according to weather conditions.
The amount-of the added water shall be adjusted to
compensate for any observed variationsin the moisture
contents. For the determination of moisture content
in the aggregates, IS 2386 (Part 3) may be referred to.
To allow for the variation in mass of aggregate due to
variation in their moisture content, suitable adjustments
in the masses of aggregates shall also be made. In the
absence of -exact data, only in the case of nominal
mixes, the amount of surface water may be estimated
from the values given in Table 10.
Table 10 Surface Water Carried by Aggregate
SI Aggregate Approximate Quantity of Surface
Percent by Mass l/m3
(1) (2) (3 (4)
0 Very wet sand 1.5 120
ii) Moderately wet sand 5.0 80
iii) Moist sand 2.5 40
iv) ‘Moist gravel or crashed rock 1.25-2.5 20-40
I)Coarser the aggregate, less the water~it will can-y.
10.2.6 No substitutions in materials used on the work
or alterations in the established proportions, except as
permitted in 10.2.4 and 10.2.5 shall be made without
additional tests to show that the quality and strength
of concrete are satisfactory.
Concrete shall be mixed in a mechanical mixer. The
mixer should comply with IS 179 1 and IS 12119. The
mixers shall be fitted with water measuring (metering)
devices. The mixing shall be continued until there is a
uniform distribution of the materials and the mass is
uniform in colour and c0nsistenc.y. If there is
segregation after unloading from the mixer, the
concrete should be remixed.
10.3.1 For guidance, the mixing time shall be at least
2 min. For other types of more efficient mixers,
manufacturers recommendations shall be followed;
for hydrophobic cement it may be decided by the
10.3.2 Workability should be checked at frequent
intervals (see IS 1199).
10.3.3 Dosages of retarders, plasticisers and
superplasticisers shall be restricted to 0.5,l .Oand 2.0
percent respectively by weight of cementitious
materials and unless a higher value is agreed upon
between the manufacturer and the constructor based
on performance test.
The formwork shall be designed and constructed so
as to remain sufficiently rigid during placing and
compaction of concrete, and shall be such as to prevent
loss of slurry from the concrete. For further details
regarding design, detailing, etc. reference may be made
to IS 14687. The tolerances on the shapes, lines and
dimensions shown in the~drawingshall be within the
limits given below:
a) Deviation from specified
dimensions of cross-section
of columns and beams
b) Deviation from dimensions
1) Dimensions in plan
0.02 times the
width of the foot-
ing in the direc-
tion of deviation
but not more than
f 0.05 times the
These tolerances apply to concrete dimensionsonly,and
not to positioning of verticalreinforcing steelor dowels.
11.2 Cleaning and ‘lhatment of Formwork
All rubbish, particularly, chippings, shavings and
sawdust shall be removed from the interior of the forms
before the concrete is placed. The face of formwork
in contact with the concrete shallbe cleaned andtreated
with form release agent. Release agents should be
applied so as to provide a thin uniform coating to the
forms without coating the reinforcement.
IS 456 : 2000
11.3 Stripping Time
Forms shall not be released until the concrete has
achieved a strength of at least twice the stress to which
the concrete may be subjected at the time of removal
of formwork. The strength referred to shall be that of
concrete using the same cement and aggregates and
admixture, if any, with the same proportions and cured
under conditions of temperature and moisture similar
to those existing on the work.
11.3.1 -Whilethe above criteria of strength shall be the
guiding factor for removal of formwork, in normal
circumstances where ambient temperature does not fall
below 15°Cand where ordinary Portland cement isused
and adequate curing is done, following striking period
may deem to satisfy the guideline given in 11.3:
Type of Formwork
Vertical formwork to columns,
Soffit formwork to slabs
(Props to be refixed
immediately after removal
Sofftt formwork to beams
(Props to be refixed
immediately after removal
Props to slabs:
1) Spanning up to 4.5 m
2) Spanning over 4.5 m
Props to beams and arches:
1) Spanning up to 6 m
2) Spanning over 6 m
For other cements and lower temperature, the
stripping time recommended above may be suitably
11.3.2 The number of props left under, their sizes and
disposition shall be such as to be able to safely carry
the full dead load of the slab, beam or arch as the case
may be together with any live load likely to occur
during curing or further construction.
11.3.3 Where the shape of the element is such that the
formwork has re-entrant angles, the formwork shall be
removed as soon as possible after the concrete has set,
to avoid shrinkage cracking occurring due to the
12 ASSEMBLY OF REINFORCEMENT
12.1 Reinforcement shall be bent and fixed in
accordance with procedure specified in IS 2502. The
high strength deformed steel bars should not be re-bent
IS 456 : 2000
or straightened without the approval of engineer-in-
Bar bending schedules shall Abeprepared for all
12.2 All reinforcement shall be placed and maintained
in the position shown in the drawings by providing
proper cover blocks, spacers, supporting bars, etc.
12.2.1 Crossing bars should not be tack-welded for
assembly of reinforcement unless permitted by
12.3 Placing of Reinforcement
Rough handling, shock loading (prior to embedment)
and the dropping of reinforcement from aheight should
be avoided. Reinforcement should be secured against
displacement outside the specified limits.
12.3.1 Tolerances on Placing of Reinforcement
Unless otherwise specified by engineer-in-charge, the
reinforcement shall be placed within the following
a) for effective depth 2oO.mm f 1Omm
b) for effective depth more than f15mm
123.2 Tolerance for Cover
Unless specified ~otherwise, actual concrete cover
should not deviate from the required nominal cover
Nominal cover as given in 26.4.1 should be specified
to all steel reinforcement including links. Spacers
between the links (or the bars where no links exist)
and the formwork should be of the same nominal size
as the nominal cover.
Spacers, chairs and other supports detailed on
drawings, together with such other supports as
may be necessary, should be used to maintain the
specified nominal cover to the steel reinforcement.
Spacers or chairs should be placed at a maximum
spacing of lm and closer spacing may sometimes be
Spacers, cover blocks should be of concrete of same
strength or PVC.
12.4 Welded JoInta or Mechanical Connections
Welded joints or mechanical connections in
reinforcement may be used but in all cases of important
connections, tests shall be made to prove that thejoints
are of the full strength of bars connected. Welding of
reinforcements shall be done in accordance with the
recommendations of IS 2751 and IS 9417.
12.5 Where reinforcement bars upto 12 mm for high
strength deformed steel bars and up to 16mm for mild
steel bars are bent aside at construction joints and
afterwards bent back into their original positions, care
should be taken to ensure that at no time is the radius
of the bend less than 4 bar diameters for plain mild
steel or 6 bar diameters for deformed bars. Care shall
also be taken when bending back bars, to ensure that
the concrete around the bar is not damaged beyond
12.6 Reinforcement should be placed and tied in such
a way that concrete placement be possible without
segregation of the mix. Reinforcement placing should
allow compaction by immersion vibrator. Within the
concrete mass, different types of metal in contact
should be avoided to ensure that bimetal corrosion does
not take place.
13 TRANSPORTING, PLACING,
COMPACTION AND CURING
13.1 Transporting and Handling
After mixing, concrete shall be transported to the
formwork asrapidly as possible by methods which will
prevent the segregation or loss of any of the ingredients
or ingress of foreign matter or water and maintaining
the required workability.
13.1.1 During hot or cold weather, concrete shall be
transported in deep containers. Other suitable methods
to reduce the loss of water by evaporation in hot
weather and heat loss in cold weather may also be
The concrete shall be deposited as nearly as practicable
in its final position to avoid rehandling. The concrete
shall be placed and compacted before initial setting of
concrete commences and should not be subsequently
disturbed. Methods of placing should be such as
to preclude segregaion. Care should be taken to
avoid displacement of reinforcement or movement
of formwork. As a general guidance, the maxi-
mum permissible free fall of concrete may be taken
Concrete should be thoroughly compacted and fully
worked around the reinforcement, around embedded
fixtures and into comers of the formwork.
13.3.1 Concrete shall be compacted using mechanical
vibrators complying with IS 2505, IS 2506, IS 2514
and IS 4656. Over vibration and under vibration of
concrete are harmful and should be avoided. Vibration
of very wet mixes should also be avoided.
Whenever vibration has to be applied externally, the
design of formwork and the disposition of vibrators
should receive special consideration to ensure efficient
compaction and to avoid surface blemishes.
13.4 Construction Joints and Cold Joints
Joints are acommon source of weakness and, therefore,
it is desirable to avoid them. If this is not possible,
their number shall be minimized. Concreting shall be
carried out continuously up to construction joints,
the position and arrangement of which shall be
indicated by the designer. Construction joints should
comply with IS 11817.
Construction joints shall be placed at accessible
locations to permit cleaning out of laitance, cement
slurry and unsound concrete, in order to create rough/
uneven surface. It is recommended to clean out laitance
and cement slurry by using wire brush on the surface
of joint immediately after initial setting of concrete
and to clean out the same immediately thereafter. The
prepared surface should be in a clean saturated surface
dry condition when fresh concrete is placed, against it.
In the case of construction joints at locations where
the previous pour has been cast against shuttering the
recommended method of obtaining a rough surface for
the previously poured concrete is to expose the
aggregate with a high pressure water jet or any other
Fresh concrete should be thoroughly vibrated near
construction joints sothat mortar from the new concrete
flows between large aggregates and develop proper
bond with old concrete.
Where high shear resistance is required at the
construction joints, shear keys may be-provided.
Sprayed curing membranes and release agents should
be thoroughly removed from joint surfaces.
Curing is the process of preventing the loss of moisture
from the concrete whilst maintaining a satisfactory
temperature regime. The prevention of moisture loss
from the concrete is particularly important if the-water-
cement ratio is low, if the cement has a high rate of
strength development, if the concrete contains
granulated blast furnace slag or pulverised fuel ash.
The curing regime should also prevent the development
of high temperature gradients within the concrete.
The rate of strength development at early ages of
concrete made with supersulphated cement is
significantly reduced at lower temperatures.
Supersulphated cement concrete is seriously affected
by inadequate curing and the surface has to be kept
moist for at least seven days.
135.1 Moist Curing
Exposed surfaces of concrete shall be kept
continuously in a damp or wet condition by ponding
or by covering with a layer of sacking, canvas, hessian
or similar materials and kept constantly wet for at least
seven days from the date of placing concrete in case
IS 456 : 2000
of ordinary Portland Cement-andat least 10days where
mineral admixtures or blended cements are used. The
period of curing shall not be less than 10 days for
concrete exposed to dry and hot weather conditions.
In the case of concrete where mineral admixtures or
blended cements are used, it is recommended that
above minimumperiods may be extended to 14 days.
13.52 Membrane Curing
Approved curing compounds may Abeused in lieu of
moist curing withthe permission of the engineer-in-
charge. Suchcompounds shallbe appliedto all exposed
surfaces of the concrete as soon as possible after the
concrete has set. Impermeable~membranes such as
polyethylene sheeting covering closely the concrete
surface may also be used to provide effective barrier
135.3 For the concrete containing Portland pouolana
cement, Portland slag cement or mineral admixture,
period of curing may be increased.
It is exceedingly difficult and costly to alter concrete
once placed. Hence, constant and strict supervision of
all the items of the construction is necessary during
the progress of the work, including the proportioning
and mixing of the concrete. Supervision is also of
extreme importance to check the reinforcement and
its placing before being covered.
13.6.1 Before any important operation, such as
concreting or stripping of the formwork is started,
adequate notice shall be given to the construction
14 CONCRETING UNDER SPECIAL
14.1 Work in Extreme Weather Conditions
During hot or cold weather, the concreting should be
done as per the procedure set out in IS 7861
(Part 1) or IS 7861 (Part 2).
14.2 Under-Water Concreting
14.2.1 When it is necessary to deposit concrete under.
water, the methods, equipment, materials and
proportions of the mix to be used shall be submitted to
and approved by the engineer-in-charge before the
work is started.
14.2.2 Under-water concrete should have a slump
recommended in 7.1. The water-cement ratio shall not
exceed 0.6 and may need to be smaller, depending on
the grade of concrete or the type of chemical attack.
For aggregates of 40 mm maximum particle size, the
cement content shall be at least 350 kg/m3of concrete.
14.23 Coffer-dams or forms shall be sufftciently tight
IS 456 : 2000
to ensure still water if practicable, and in any case to
reduce the flow of water to less than 3 mAninthrough
the space into which concrete is to be deposited.
Coffer-dams or forms in still water shall be sufficiently
tight to prevent loss of mortar through the walls.
De-watering by pumping shall not be done while
concrete is being placed or until 24 h thereafter.
14.2.4 Concrete cast under water should not fall freely
through the water. Otherwise it may be leached and
become segregated. Concrete shall be deposited,
continuously until it is brought to the required height.
While depositing, the top surface shallbe kept as nearly
level as possible and the formation of seams avoided.
The methods to be used for depositing concrete under
water shall be one of the following:
a>Tremie-The concrete is placed through vertical
pipes the lower end of which is always inserted
sufficiently deep into the concrete which has
been placed ~previously but has not set. The
concrete emerging from the pipe pushes the
material that has already been placed to the side
and upwards and thus does not come into direct
contact with water.
When concrete is to be deposited under water
by means of tremie, the top section of the tremie
shall be a hopper large enough to hold one entire
batch of the mix or the entire contents the
transporting bucket, if any. The tremie pipe shall
be not less than 200 mm in diameter and shall
be large enough to allow a free flow of concrete
and strong enough to withstand the external
pressure of the water in which it~issuspended,
even if a partial vacuum develops insidethe pipe.
Preferably, flanged steel pipe of adequate
strength for the job should be used. A separate
lifting device shall be provided for each tremie
pipe with its hopper at the upper end. Unless
the lower end of the pipe is equipped with an
approved automatic check valve, the upper end
of the pipe shall be plugged with a wadding of
the gunny’sacking or other approved material
before delivering the concrete to the tremie pipe
through the hopper, so that when the concrete is
forced down from the hopper to the pipe, it will
force the plug (and along with it any water in
the pipe) down the pipe and out of the bottom
end, thus establishing a continuous stream of
concrete. It will be necessary to raise slowly the
tremie in order to cause a uniform flow of the
concrete, but the tremie shall not be emptied so
that water enters the pipe. At all times after the
placing of concrete is started and until all the
concrete is placed, the lower end of the tremie
pipe shall be below the top surface of the plastic
concrete. This will cause the concrete to build
up from below instead of flowing out over the
surface, and thus avoid formation of laitance
layers. If the charge in the tremie is lost while
depositing, the tremie shall be raised above the
concrete surface, and unless sealed by a check
valve, it shall be re-plugged at the top end, as at
the beginning, before refilling for depositing
Direct placement with pumps-As in the case
of the tremie method, the vertical end piece of
the pipe line is always inserted sufficiently deep
into the previously cast concrete and should not
move to the side during pumping.
c) Drop bottombucket -The top of the bucket shall
be covered with a canvas flap. The bottom doors
shall open freely downward and outward when
tripped.The bucket shallbe filled completely and
lowered slowly to avoid backwash. The bottom
doors shall not be opened until the bucket rests
on the surface upon which the concrete is to be
deposited and when discharged, shall be
withdrawn slowly until well above the concrete.
Bags - Bags of at least 0.028 m3capacity of
jute or other coarse cloth shall be filled about
two-thirds full of concrete, the spare end turned
under so that bag is square ended and securely
tied. They shall be placed carefully in header
and stretcher courses so that the whole mass is.
interlocked. Bags used for this purpose shall be
free from deleterious materials.
Grouting-A series of round cages made from
50 mm mesh of 6 mm steel and extending over
the full height to be concreted shall be prepared
and laid vertically over the area to~beconcreted
so that the distance between centres of the cages
and also to the faces of the concrete shall not
exceed one metre. Stone aggregate of not less
than 50 mm nor more than 200 mm size shall be
deposited outside the steel cages over the full
area and height to be concreted with due care to
prevent displacement of the cages.
A stable 1:2 cement-sand grout with a water-
cement ratio of not less than 0.6 and not more
than 0.8 shall be prepared in a mechanical mixer
and sent down under pressure (about 0.2 N/mm*)
through 38 to 50 mm diameter pipes terminating
into steel cages, about 50 mm above the bottom ,.
of the concrete. As the grouting proceeds, the
pipe shall be raised gradually up to a height of
not more than 6 000 mm above its starting level
after which it may be withdrawn and placed into
the next cage for further grouting by the same
After grouting the whole area for a height of
about 600 mm, the same operation shall be
repeated, if necessary, for the next layer of
600 mm and so on.
The amount of grout to be sent down shall be
sufficient to fill all the voids which may be either
ascertained or assumed as 55 percent of the
volume to be concreted.
14.2.5 To minimize the formulation of laitance, great
care shall be exercised not to disturb the concrete as
far as possible while it is being deposited.
15 SAMPLING AND STRENGTH OF
DESIGNED CONCRETE MIX
Samples from fresh concrete shall be taken as per
IS 1199 and cubes shall be made, cured and tested at
28 days in accordance with IS 516.
15.1.1 In order to get a relatively quicker idea of the
quality of concrete, optional tests on beams for
modulus of rupture at 72 + 2 h or at 7 days, or
compressive strength tests at 7 days may be carried
out in addition to 28 days compressive strength test.
For this purpose the values should be arrived at based
on actual testing. In all cases, the 28 days compressive
strength specified in Table 2 shall alone be the criterion
for acceptance or rejection of the concrete.
15.2 Frequency of Sampling
15.2.1 Sampling Procedure
A random sampling procedure shall be adopted to
ensure that each concrete batch shall have a reasonable
chance of being tested that is, the sampling should be
spread over the entire period of concreting and cover
all mixing units.
The minimum frequency of sampling of concrete of
each grade shall be in accordance with the following:
Quantity of Concrete in the Number of Samples
I- 5 1
6- 15 2
16- 30 3
5 1 and above 4 plus one
for -each additional
50 m3 or part thereof
NOTE-At least one sample shall be taken from each Shift.
Where concrete is produced at continuous production unit, such
as ready-mixed concrete plant, frequency of’sampling may be
agreed upon mutually by suppliers and purchasers.
15.3 Test Specimen
Three test specimens shall be made for each sample
IS 456 : 2000
for testing at 28 days. Additional samples may be
required for various purposes such as to determine the
strength of concrete at 7 days or at the time of striking
the formwork, or to determine the duration of curing,
or to check the testing error. Additional samples may
also be required for testing samples cured by
accelerated methods as described in IS 9103. The
specimen shall be tested as described in IS 516.
15.4 Test Results of Sample
The test results of the sample shall be the average of
the strength of three specimens. The individual
variation should not be more than +15 percent of the
average. If more, the test results of the sample are invalid.
16 ACCEPTANCE CRITERIA
16.1 Compressive Strength
The concrete shall be deemed to comply with the
strength requirements when both the following
condition are met:
a) The mean strength determined from any group
of four consecutive test results compiles with
the appropriate limits in co1 2 of Table 11.
b) Any individual test result complies with the
appropriate limits in co1 3 of Table 11.
16.2 FIexural Strength
When both the following conditions are met, the
concrete complies with the specified flexural strength.
The mean strength determined from any group
of four consecutive test results exceeds the
specified characteristic strength by at least 0.3
The strength determined from any test result is
not less than the specified characteristic strength
less 0.3 N/mmz.
16.3 Quantity of Concrete Represented by
Strength Test Results
The quantity of concrete represented~by a group of
four consecutive test-results shall include the batches
from which the first and last samples were taken
together with all intervening batches.
For the individual test result requirements given in
co1 2 of Table 11 or in item (b) of 16.2, only the
particular batch from which the sample was taken shall
be at risk.
Where the mean rate of sampling is not specified the
maximum quantity of concrete that four consecutive
test results represent shall be limited to 60 m3.
16.4 If the concrete is deemed not to comply persuant
to 16.3, the structural adequacy of the parts affected
shall be investigated (see 17) and any consequential
action as needed shall be taken.
IS 456 : 2000
16.5 Concrete of each grade shall be assessed
16.6 Concrete is liable to be rejected if it is porous
or honey-combed, its placing has been interrupted
without providing a proper construction joint, the
reinforcement has been displaced beyond the
tolerances specified, or construction tolerances have
not been met. However, the hardened concrete
may be accepted after carrying out suitable
remedial measures to the satisfaction of the engineer-
there is a system to verify that the quality is
satisfactory in individual parts of the structure,
especially the critical ones.
Immediately after stripping the formwork, all
concrete shall be carefully inspected and any defective
work or small defects either removed or made good
before concrete has thoroughly hardened.
17 INSPECTION AND TESTING OF
In case of doubt regarding the grade of concrete used,
either due to poor workmanship or based on results of
cube strength tests, compressive strength tests of
concrete on the basis of 17.4 and/or load test (see 17.6)
may be carried out.
17.1 Inspection 17.4 Core Test
To ensure that the construction complies with the
design an inspection procedure should be set up
covering materials, records, workmanship and
17.1.1 Tests should be made on reinforcement and
the constituent materials of concrete in accordance with
the relevant standards. Where applicable, use should
be made of suitable quality assurance schemes.
17.4.1 The points from which cores are to be taken
and the number of cores required shall be at the
discretion of the engineer-in-charge and .shall be
representative of the whole of concrete concerned.
,In no case, however, shall fewer thau three cores be
17.4.2 Cores shall be prepared and tested as described
in IS 516.
17.1,.2 Care should be taken to see that: 17.4.3 Concrete in the member represented by a core
test shall be considered acceptable if the average
equivalent cube strength of thecores is equal to at least
85 percent of the cube strength of the grade of concrete
specified for the corresponding age and no individual
core has a strength less than 75 percent.
17.5 In case the core test results do not satisfy the
requirements of 17.4.3 or where such tests have not
been done, load test (17.6) may be resorted to.
design and detail are capable of being executed
to a suitable standard, with due allowance for
there are clear instructions on inspection
there are clear instiuctions on permissible
elements critical to workmanship, structural
performance, durability and appearance are
17.6 Loa+ Tests for Flexural Member
17.6.1 Load tests should be carried out as soon as
Table 11 Characteristic Compressive Strength Compliance Requirement
(Clauses 16.1 Md 16.3)
Mean of the Group of
2 fa +0.825Xestablished
off to neatest0.5 N/mm*)
f, + 3 N/I&,
2 fe + 0.825x estublished
off to nearest0.5 N/mm*)
f”’+ 4 N/mm*,whichever
2 f,” Nlmm’
NOTE-In the ubsenceof establishedv&e of standurddeviution,the vuluesgiven inTable8 maybeassumed,andattemptshouldbe
madeto obtainresultsof 30 samplesusearlyuspossible to estublishthe vulueof stundurddeviation.
IS 456 : 2000
possible after expiry of 28 days from the time of placing
17.6.2 The structure should be subjected to a load equal
to full dead load of the structure plus 1.25 times the
imposed load for a period of 24 h and then the imposed
load shall be removed.
NOTE-Dead load includes self weight of the structural
members plus weight of finishes and walls or partitions, if -any,
as considered in the design.
17.6.3 The deflection due to imposed load only shall
be recorded. If within 24 h of removal of the imposed
loa< the structure does not recover at least 75 percent
of the deflection under superimposed load, the test may
be repeated after a lapse of 72 h. If the recovery is less
than 80 percent, the structure shall be deemed to be
188.8.131.52 If the maximum deflection in mm, shown
during 24 h under load is less than 4012/D, where 1is
the effective span in m; and D, the overall depth of the
section in~mm, it is not necessary for the recovery to
be measured and the recovery provisions of 17.6.3 shall
17.7 Members Other Than Flexural Members
Members other than flexural members should be
preferably investigated by analysis.
17.8 anon-destructive Tests
Non-destructive tests are used to obtain estimation of
the properties of concrete in the structure. The methods
adopted include ultrasonic pulse velocity [see IS 133 11
(Part l)] and rebound hammer [IS 13311 (Part 2)],
probe penetration, pullout and maturity. Non-
destructive tests provide alternatives to core tests for
estimating the strength of concrete in a structure, or
can supplement the data obtained from a limited
number of cores. These methods are based on
measuring a concrete property that bears some
relationship to strength. The accuracy of these methods,
in part, is determined by the degree of correlation
between strength and the physical quality measured
by the non-destructive tests.
Any of these methods may be adopted, in which case the
acceptance criteria shall be agreed upon prior to testing.